#------------------------------------------------------------------------------
#$Date: 2026-08-01 22:49:11 +0200 (Sat 01 de Aug de 2026) $
#$Revision: 306707 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/07/4300747.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4300747
loop_
_publ_author_name
'SeethaLekshmi, Nanappan'
'Pedireddi, V. R.'
_publ_section_title
;
 First Study of Metal Hybrids of Boronic Acids: Second-Sphere
 Coordination Networks in the Structures of 4-Carboxyphenylboronic
 Acid with Some Transition Metals
;
_journal_coden_ASTM              INOCAJ
_journal_issue                   6
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2400
_journal_page_last               2402
_journal_paper_doi               10.1021/ic052100h
_journal_volume                  45
_journal_year                    2006
_chemical_formula_moiety         ' [Ni (H2 O)6], 4(H2 O), 2(C7 H6 B1 O4)'
_chemical_formula_sum            'C14 H32 B2 Ni O18'
_chemical_formula_weight         568.73
_chemical_name_common
;
4-Carboxylato-phenylboronic acid nickel(II) hexahydrate
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                97.89(4)
_cell_angle_beta                 92.05(5)
_cell_angle_gamma                108.55(4)
_cell_formula_units_Z            1
_cell_length_a                   6.781(2)
_cell_length_b                   9.572(3)
_cell_length_c                   9.824(3)
_cell_measurement_temperature    133(2)
_cell_volume                     596.7(3)
_diffrn_ambient_temperature      133(2)
_exptl_crystal_density_diffrn    1.583
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               4300747
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ni1 Ni 0.0000 0.5000 0.0000 0.01516(14) Uani 1 2 d S . .
O90 O 0.1403(3) 0.6167(2) 0.1905(2) 0.0249(4) Uani 1 1 d . . .
O91 O 0.0407(3) 0.31813(19) 0.06351(18) 0.0195(4) Uani 1 1 d . . .
H912 H -0.055(5) 0.232(3) 0.048(3) 0.022(7) Uiso 1 1 d . . .
H902 H 0.177(5) 0.572(3) 0.234(3) 0.027(9) Uiso 1 1 d . . .
H901 H 0.168(4) 0.707(4) 0.221(3) 0.030(8) Uiso 1 1 d . . .
O92 O 0.2856(3) 0.5452(2) -0.0806(2) 0.0211(4) Uani 1 1 d . . .
H922 H 0.277(6) 0.542(4) -0.155(4) 0.047(12) Uiso 1 1 d . . .
O93 O 0.2645(4) 0.5839(2) 0.6423(2) 0.0267(5) Uani 1 1 d . . .
O94 O 0.1547(3) 0.4253(2) 0.3817(2) 0.0260(4) Uani 1 1 d . . .
B1 B 0.2786(4) 0.0616(3) -0.6365(3) 0.0149(5) Uani 1 1 d . . .
C1 C 0.2793(4) 0.0659(3) -0.4773(2) 0.0159(5) Uani 1 1 d . . .
C2 C 0.2268(4) -0.0663(3) -0.4202(2) 0.0187(5) Uani 1 1 d . . .
H2 H 0.186(4) -0.158(3) -0.485(3) 0.025(7) Uiso 1 1 d . . .
C3 C 0.2340(4) -0.0637(3) -0.2793(2) 0.0181(5) Uani 1 1 d . . .
H3 H 0.200(4) -0.152(3) -0.243(3) 0.023(7) Uiso 1 1 d . . .
C4 C 0.2918(3) 0.0713(2) -0.1888(2) 0.0149(5) Uani 1 1 d . . .
C5 C 0.3413(4) 0.2036(3) -0.2435(2) 0.0180(5) Uani 1 1 d . . .
H5 H 0.384(4) 0.295(3) -0.185(3) 0.019(7) Uiso 1 1 d . . .
C6 C 0.3358(4) 0.2007(3) -0.3857(2) 0.0188(5) Uani 1 1 d . . .
H6 H 0.381(5) 0.295(3) -0.419(3) 0.032(8) Uiso 1 1 d . . .
C7 C 0.3012(3) 0.0728(2) -0.0350(2) 0.0158(5) Uani 1 1 d . . .
O11 O 0.2232(3) -0.07033(18) -0.72206(18) 0.0197(4) Uani 1 1 d . . .
H11 H 0.231(6) -0.065(4) -0.807(4) 0.070(13) Uiso 1 1 d . . .
O12 O 0.3378(3) 0.19459(17) -0.68626(17) 0.0185(4) Uani 1 1 d . . .
H12 H 0.355(6) 0.198(4) -0.787(4) 0.065(12) Uiso 1 1 d . . .
O71 O 0.2435(3) -0.05055(17) 0.01187(17) 0.0207(4) Uani 1 1 d . . .
O72 O 0.3645(2) 0.19989(16) 0.04521(16) 0.0171(4) Uani 1 1 d . . .
H911 H 0.146(5) 0.303(3) 0.045(4) 0.038(10) Uiso 1 1 d . . .
H921 H 0.386(7) 0.627(5) -0.059(4) 0.066(12) Uiso 1 1 d . . .
H942 H 0.186(5) 0.360(4) 0.355(4) 0.038(10) Uiso 1 1 d . . .
H932 H 0.362(6) 0.650(4) 0.640(4) 0.040(11) Uiso 1 1 d . . .
H941 H 0.202(7) 0.475(5) 0.472(6) 0.108(18) Uiso 1 1 d . . .
H931 H 0.191(12) 0.588(8) 0.649(8) 0.16(4) Uiso 1 1 d . . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ni1 O91 2.0217(18) . ?
Ni1 O91 2.0217(18) 2_565 ?
Ni1 O92 2.0580(19) 2_565 ?
Ni1 O92 2.0580(19) . ?
Ni1 O90 2.0680(19) . ?
Ni1 O90 2.0680(19) 2_565 ?
B1 O11 1.352(3) . ?
B1 O12 1.371(3) . ?
B1 C1 1.558(3) . ?
C1 C6 1.402(3) . ?
C1 C2 1.402(3) . ?
C2 C3 1.381(3) . ?
C3 C4 1.397(3) . ?
C4 C5 1.391(3) . ?
C4 C7 1.507(3) . ?
C5 C6 1.392(3) . ?
C7 O71 1.276(3) . ?
C7 O72 1.291(3) . ?
